Installation Guides

At Unique Design Solutions, we put a lot of care into crafting and delivering your material. In order to help make sure that your project and tile installation are executed successfully, we have partnered with the experts at Laticrete International to provide rock solid recommendations on suitable setting and grouting products for our wide variety of material options, as well as helpful tile installation tips and resources.

Mirror tiles are particularly susceptible to oxidation from cement-based adhesive mortars. This can adversely impact the appearance of your project. We recommend the use of LATAPOXY 300, an epoxy-based adhesive mortar. In any case, be sure to use an epoxy-based adhesive mortar (or similar alternative) and not a cement-based adhesive mortar when installing mirror tiles.

See the Tile Council of North America (TCNA) handbook for complete details regarding specific methods of preparing substrates for tile installation.

Crack Isolation

All existing substrates cracks as well as any area susceptible to future surface cracking requires the installation of a crack isolation membrane meeting ANSI 118.12.

Wet Areas

Installation of a waterproofing membrane meeting ANSI 118.10 prior to installation is recommended for wet areas. Steam Rooms (continuous use) require a waterproofing and vapor retarding membrane with a perm rating of .05 perms or less.

Setting

Prior to installation, dry lay all material to inspect for quality and to determine the best blend. All materials must be acclimated prior to installation, and air and surface temperature should be between 50⁰F and 80⁰F during installation. Be sure to clean tiles to remove any dust, dirt or packing contaminants before installation.

Select a notch trowel size that will achieve the proper coverage rate and maintain a minimum bed thickness of 3/32”. A minimum coverage of 95% is required. Per ANSI A108.5, apply mortar to the substrate using a notched trowel, and place tiles while material is wet and offers transfer. Once setting materials have adequately set (see product specifications for dry time) grouting can proceed. Before grouting, a grout release product may be advisable depending on material (ex: natural stone).

Prior to commencing installation, the Contractor is to examine substrates and advise of all existing conditions and surface contamination which will require correction. Before starting, substrates are to be cleaned to remove concrete curing compounds, sealers, soil, mortar, dirt, dust, paint, etc.

Mixing

Mix according to printed product instructions included with each LATICRETE® product package.

Fill all substrate cracks, cold joints and control joints to a smooth finish using a LATICRETE latex-fortified thin-set. Alternatively, a liberal coat of HYDRO BAN applied with a paint brush or trowel may be used to fill in non-structural joints and cracks.

Pre-Treat Coves and Floor/Wall Intersections

Fill all substrate coves and floor/wall transitions to a smooth finish and changes in plane using a LATICRETE latex-fortified thin-set. Alternatively, a liberal coat of HYDRO BAN applied with a paint brush or trowel may be used to fill in cove joints and floor/wall transitions <1/8” (3mm) in width.

Pre-Treat Drains

Drains must be of the clamping ring type, with weepers as per ASME A112.6.3. Apply a liberal coat of HYDRO BAN around and over the bottom half of drain clamping ring. Cover with a second liberal coat of HYDRO BAN. When the HYDRO BAN dries, apply a bead of LATICRETE LATASIL™ where the HYDRO BAN meets the drain throat. Install the top half of drain clamping ring.

Pre-Treat Penetrations

Allow for a minimum 1/8” (3mm) space between drains, pipes, lights, or other penetrations and surrounding tile, stone or brick. Pack any gaps around pipes, lights or other penetrations with a LATICRETE latex-fortified thin-set. Apply a liberal coat* of HYDRO BAN around penetration opening. Cover the first coat with a second liberal coat of LATICRETE® HYDRO BAN®. Bring HYDRO BAN up to level of tile or stone. When HYDRO BAN has dried to the touch seal with LATICRETE LATASIL™.

Main Application

Allow any pre-treated areas to dry to the touch. Apply a liberal coat of HYDRO BAN with a paint brush or heavy napped roller over substrate including pre-treated areas and allow to dry to the touch. Apply a second liberal coat of HYDRO BAN over the first coat. Allow the top coat of HYDRO BAN dry to the touch approximately. When the top coat has dried, inspect the surface for pinholes, voids, thin spots or other defects. HYDRO BAN will dry to an olive green color when fully cured. Use additional HYDRO BAN to seal any defects.

Movement Joints

Apply a liberal coat of HYDRO BAN, approximately 8” (200mm) wide over the necessary areas. Then embed and loop the 6” (150mm) wide LATICRETE Waterproofing/Anti-Fracture Fabric and allow the HYDRO BAN liquid to bleed through. Immediately apply a second coat of HYDRO BAN.

Provide protection for newly installed membrane, even if covered with a thin-bed tile, stone or brick installation against exposure to rain or other water for a minimum of 2 hours at 70°F (21°C). For temperatures between 45°F and 69°F (7°C to 21°C) allow a minimum 24 hour cure period.

Flood Testing

Allow membrane to cure fully before flood testing, typically a minimum 2 hours at 70°F (21°C) and 50% relative humidity. For temperatures between 50°F and 69°F (10°C to 21°C) allow a minimum 24 hour cure period prior to flood testing.

Install LATICRETE® 254 Platinum in compliance with current revisions of ANSI A108.02, A108.1B and ANSI A108.5. Use the appropriate trowel notch size to ensure proper bedding of the tile selected. Work the thinset into good contact with the substrate and comb with notched side of trowel. Spread only as much thinset as can be covered while the mortar surface is still wet and tacky. When installing over metal or other unusual substrates, use LATAPOXY® 300 Epoxy Adhesive. Allow installation to set until firm. Clean excess latex Portland cement mortar from tile face and joints between pieces.

Wall TileInstallation

Thin Bed Method

Install LATICRETE 254 Platinum (must use for Exterior Applications), with current revisions of ANSI A108.02 (3.11), A108.1B, ANSI A108.5 and ANSI A108.19. Select an appropriately-sized notched trowel that will provide full bedding and coverage. Use flat side of trowel to apply/key in the adhesive mortar into full contact with the substrate. Immediately following, apply mortar with notched side of trowel. Spread only as much mortar as can be covered while the mortar surface is still wet and tacky. Mortar is to be applied to the tile backs to key in the mortar with the flat side of the trowel then bed the tiles with a rubber mallet to achieve a minimum 95% continuous coverage for exterior applications, and coverage in accordance with ANSI A108.19.15.2 for interior vertical applications. Periodically remove a freshly set tile to validate coverage. Clean excess latex Portland-cement mortar from tile face and joints between pieces, immediately. Allow installation to cure for minimum 24 hours at 70° F (21° C), prior to grouting.

NOTE: LATICRETE® PERMACOLOR® Select is an advanced, high performance cement grout that offers the industry’s first dispensable dry pigment solution. LATICRETE PERMACOLOR Select is designed for virtually all types of residential and commercial installations and offers optimum performance on the most demanding exterior or interior applications. Easy to mix, grout and clean, LATICRETE PERMACOLOR Select is fast setting and is suitable for joints 1/16” to ½” (1.5mm – 12mm) wide on floors or walls.

Surface Preparation

Before starting to grout, remove spacers and debris in grout joints and remove dust and dirt using a wet sponge. Do not leave water standing in joints. Substrate temperature must be between 40°F (4°C) and 90°F (32°C). Apply grout release or sealer if necessary. Refer to TDS 400 Grout Guide for more information on grouting.

Mixing

Use approximately 2 – 2.25 quarts (1.9 L – 2.1 L) of clean potable water for 2 LATICRETE PERMACOLOR Select Color Packs and 25 lbs (11.3 kg) of LATICRETE PERMACOLOR Select Grout Base. Do not use with 1776 Grout Enhancer or any other latex additive. Place water in a clean mixing container. Remove Color Packs from the cardboard container as well as the protective plastic sleeve. The internal bag is a water-dispersible pack – when using the 25 lbs. (11.3 kg) bag of LATICRETE PERMACOLOR Select, drop both color packs directly to water in clean mixing container. Mix with a drill mixer until pigment is dispersed evenly in container and the dispersible pack is no longer visible. Add LATICRETE PERMACOLOR Select Base. Mix with a slow speed drill mixer (300 rpm) for 1 minute. Wait for 5 minutes and remix with drill for 1 minute. If using the 12.5 lb. bag, drop only one color pack into 1 – 1.1 quarts (.8L – 1.0 L) of clean water.

Application

Clean tile surface with a damp sponge. Spread with a sharp, firm rubber grout float or wall float for narrow wall joints. To remove excess grout hold the float at a 90° angle and pull it at a 45° angle diagonally across the joints to avoid pulling out the material.

Note: If the grout begins to stiffen during installation, remix with drill mixer for 10–15 seconds. DO NOT ADD MORE WATER.

Cleaning

For first cleaning wait approximately 35 – 40 minutes at 70°F (21°C). Wider joints or cooler temperatures may extend wait time. Begin initial cleaning by lightly wiping down entire area to be cleaned with a damp sponge. Wash with a damp sponge (not wet). Work diagonally to the joints. Allow to dry 3 hours at 70°F (21°C). For second cleaning use a damp sponge or dry cloth to remove remaining grout haze.Note: If grout is to be sealed, LATICRETE generally recommends waiting a minimum of a 72 hours at 70°F (21°C) prior to sealing LATICRETE PERMACOLOR Select, with a LATICRETE STONETECH® PROFESSIONAL Sealer.

Stain-Resistant Epoxy Grout Installation

Follow manufacturer‘s recommendations for minimum cure time prior to grouting.Substrate temperature must be 40-95°F (4-35°C). Verify joints are free of dirt, debris or grout spacers. Sponge or wipe dust/dirt off tile faces and remove water standing in joints. Apply grout release to face of tile if applicable. Cut open pouch and pour SPECTRALOCK PRO Premium Grout Part A Liquid into a clean mixing pail. Then open pouch and pour SPECTRALOCK PRO Premium Grout Part B Liquid into the mixing pail. Mix by hand or with a slow speed mixer until the two liquids are well blended. Then, while mixing, add SPECTRALOCK PRO Premium Grout Part C Powder and blend until uniform.

Install SPECTRALOCK PRO Premium Grout in compliance with current revisions of ANSI A108.02 and ANSI A108.6. Spread using a sharp edged, hard rubber float and work grout into joints, packing joints full and free of voids/pits. Then hold float face at a 90° angle to grouted surface and use float edge to "squeegee" off excess grout. Once excess grout is removed, a thin film/haze will be left. Initial cleaning of the remaining film/haze can begin approximately 20-30 minutes after grouting.Begin by mixing cleaning additive packet with 2 gallons (7.6 L) of clean water in a clean bucket to make cleaning solution. Dip a clean sponge into the bucket and then wring out cleaning solution until sponge is damp.Using a circular motion, lightly scrub grouted surfaces with the damp sponge to dissolve grout film/haze. Then drag sponge diagonally over the scrubbed surfaces to remove froth. Rinse sponge frequently and change cleaning solution at least every 50 ft2 (4.7m2). Discard sponges as they become "gummy" with residue.Within one (1) hour of finishing first cleaning, clean the same area again following the same procedure but utilizing a clean white scrub pad and fresh cleaning solution. Rinse scrub pad frequently. Drag a clean sponge diagonally over the scrubbed surfaces to remove froth. Use each side of sponge only once before rinsing and change cleaning solution at least every 50 ft2 (4.7m2).

The curing of latex and Portland cement-based materials is retarded by low temperatures and finished work should be protected for an extended period of time. Typically, for every 18º F below 70º F (10ºC below 21ºC), latex and Portland cement-based materials take twice as long to cure.

As a professional courtesy, LATICRETE does offer technical services free of charge. LATICRETE does not have any express or implied contractual obligation or duty to provide those technical services. The user maintains all responsibility for verifying the applicability and suitability of the technical service or information provided by LATICRETE representatives. Moreover, technical service site visits and consultations do not constitute express or implied approval by LATICRETE of product use or other construction means and methods. By providing technical services, LATICRETE does not undertake to perform any duty owed by the user to any third party, and no third party should rely on LATICRETE providing technical services.